Tensile Testing of Plastics ISO 527-1
ISO 527-1 tensile testing provides key data on tensile strength, modulus and elongation of plastics at ambient, elevated or reduced temperatures.
Scope: Tensile tests measure the force required to break a plastic sample specimen and the extent to which the specimen stretches or elongates to that breaking point.
Specimens are placed in the grips of the universal tester at a specified grip separation and pulled until failure. For ISO 527 the test speed is typically 5 or 50mm/min for measuring strength and elongation and 1mm/min for measuring modulus. An extensometer is used to determine elongation and tensile modulus.
Elevated or Reduced temperature test procedure:
A thermal chamber is installed on the universal test machine. The chamber is designed to allow the test mounts from the base and crosshead of the universal tester to pass through the top and bottom of the chamber. Standard test fixtures are installed inside the chamber, and testing is conducted inside the controlled thermal environment the same as it would be at ambient temperature. The chamber has internal electric heaters for elevated temperatures and uses external carbon dioxide gas as a coolant for reduced temperatures. The size of the chamber places a limitation on the maximum elongation that can be reached, and extensometers are generally limited to no more than 200° C.
Specimen size: The most common specimen for ISO-527 is the ISO-3167 Type 1A multipurpose specimen.
The following calculations can be made from tensile test results:
- Tensile strength (at yield and at break)
- Tensile modulus
- Elongation and percent elongation at yield
- Elongation and percent elongation at break
Need help or have a question?
- Wilton UK:
- +44 1642 435 788
- +31 88 126 8888
- +65 6805 4800
- 0800 5855888
- +49 711 27311 152
- +41 61 686 4800
- 01 800 5468 3783
- +52 55 5091 2150
- +55 11 2322 8033
- +61 1300 046 837
- +91 22 4245 0207